Polymers. Long string like molecules give rise to universal properties in dynamics as well as in structure – properties of importance when dealing with: Pure polymers and polymer solutions & mixtures Composites (reinforced plastics)
Long string like molecules give rise to universal properties in dynamics as well as in structure – properties of importance when dealing with:
Pure polymers and polymer solutions & mixtures
Composites (reinforced plastics)
Biological macromolecules (DNA, F-actin, cellulose, natural rubber etc.)
With simple models we will be able to:
Syntetic polymers always show a distribution in molecular weights.
number average :
(ni and wi are number and weight fractions, respectively, of molecules with molar mass Mi)
The polydispersity index is given by Mw /Mn
10 chains of 100 molecular weight
20 chains of 500 molecular weight
40 chains of 1000 molecular weight
5 chains of 10000 molecular weight
Stereo isomers of poly propylene
Tacticity determines ability to form crystals: Disordered, atactic polymers form glasses.
Newman projections of the C-C bond in the middle of butane.
Rotation about σ bonds is neither completely rigid nor completely free.
A polymer molecule with 10000 carbons have 39997 conformations
The energy barrier between gauche and trans is about 2.5 kJ/mol
RT~8.31*300 J/mol~2.5 kJ/mol
For a polymer chain model;
The chain end-to-end vector R “describes” a coil made up of N jump vectors ai.
R is made up of N jump vectors ai . The average of all conformational states of the polymer is <R>=0
The simplest non-zero average is the mean-square end to end distance <R2>
(A matrix of dot-products where the diagonal represents i=j and off axis elements i≠j)
For a freely jointed chain the average of the cross terms above is zero and we recover a classical random walk: <R2>=Na2
The rms end to end distance <R2>1/2=N1/2a
An ideal polymer chain with 106 repeat units (not unusual), each unit about 6Å will have:
The rms end to end distance <R2>1/2=N1/2a
The random walk and the steric limitations makes the polymer coils in a polymer melt or in a polymer glass “expanded”.
However, the overlap between molecules ensure space filling
The distribution of end-to-end distances (R) in an ensemble of random polymer coils is Gaussian. The probability function is:
The probability decreases monotonically with increasing R (one end is attached at origo). The radial distribution g(R) is obtained by multiplying with 4πR2
Adopted from Gedde; Polymer Physics
ln P(R) = ln Ω; where Ω=statistical weight
Since S=kblnΩ we have an expression for the entropy of a Gaussian coil:
Entropy decreases with stretching (increasing order)
F=U-TS=>The “Entropic Spring” with a spring constant:
OBS: dF/dR Increases with T, decreases with N – not like a traditional spring which depends on U!
Recall that :
The correlation between bond vectors “dies” with increasing separation:
Thus the sum over bond angles converges to a finite number and we have:
Flory Characteristic Ratio
After renormalisation this relation holds for all flexible linear polymers!
Instead of <R2>1/2=aN1/2 we will have
Experiments tells us that in general: v~0.6
Consider a cube containing N segments of a polymer
V=r3 where r is the radius of gyration.
The concentration of segments is c~N/r3
Each segment with volume ע “stuffed” into the cube reduces the entropy with –kbעN/V = -kbעN/r3 (for small x;ln(1-x)~lnx)
The result is a positive contribution to F; Frep= kbעTN/r3 (expansion of the coil)
From before; Coiling reduces the entropy; Fel=kbT3R2/2Na
The total free energy F is the sum of the two contributions!
Search for equilibrium!
In dilute polymer solutions the excluded volume effect is large. (OBS Theta cond. Later)
When chains start to overlap the expanding force on a single coil will be reduced
In a polymer melt the concentration of segments is uniform due to space filling. No swelling!
A stress σ0is applied at time t=0 and held constant. The strain e(t) is followed over time. The creep compliance J(t) is given by:
e(t)= σ0 J(t)
A strain e0 is applied at t=0 and held constant. The stress σ(t) is followed over time. The stress relaxation modulus G(t) is given by:
If a sinusoidal strain is applied: e(t)=e0cos(ωt) the resulting stress is given by:
σ(t) = e0[G’(ω) cos(ωt) – G’’(ω) sin(ωt)]
The complex modulus, G*= G’(ω) + G’’(ω) is given by a Fourier transform of G(t).
G’ gives elastic response, G’’ the viscous responce
All relaxing modes in a polymer melt or a solution have the same T-dependence. Therefore:
G(t,T) = G(aTt, T0)
log aT = -[C1(T-T0)]/[C2+T-T0]
“Quasi-universal” values of C1 and C2 are 17.4 and 51.6 K, respectively
The superposition principle help us building larger data set over timescales/temperatures otherwise out of reach
The stress relaxation G(t) for two polymers (homologues) with different molecular weights.
At short time the curves are identical.
At intermediate times we have a plateau with a constant modulus – the plateau modulus.
The plateau ends at a terminal time τT which depends strongly on molecular weights (N) according to a power law τT~Nm where the exponent m ≈ 3.4
Two Q’s arises: 1) Why is m ≈ 3.4 almost universal? 2) why do we have an almost purely elastic behaviour at the plateau?
Every segment in the tube have a mobility, μseg restricted by the surrounding “resistance”.
The tube with N segments have a mobilty, μtube= μseg/N
Brownian motion within the tubes confinement – use Einstein relation to calculate a Diffusion coefficient =>
=> Dtube=kbT μtube=kbT μseg/N
A polymer escapes from its own tube of length L after a time τT
Close to the exp. results!
In a similar way as we explained the elastic behaviour at very short times for all simple liquids “as a glassy state” we can explain the rubber plateau in a qualitative way as a signature of entanglements.
It can be shown that in a rubber, a cross linked polymer (see Ch. 5.4), the elastic modulus depends on the average molecular mass between cross-links Mx, R ,T and the density ρ:
Adopting an identical relation and treating the entanglements as temporary cross-links with a lifetime of the order of τT we can calculate an average mass of the molecular mass between the entanglements (Me).
Polymers in solutions are a major topic in polymer science – applied as well as theoretical.
Following the arguments from chapter 3 we derive an expression for the mixing when new p-s contacts are made and old p-p and s-s contacts are lost:
The internal energy U will change with the addition of polymer to a solvent:
Combining the new expression for ΔUint with the previous for coil swelling:
The value of x determines if excluded volume effects are dominating or whether they are counteracted by the p-s interaction:
When x=1/2 the two energies cancel and we have a “theta solvent” with pure random walk conformation!
When x<1/2 the coil is swollen (A good solvent; Clint E?)
When x>1/2 the coil forms a globule (A bad or poor solvent)